Chrome plating

Manual cleaning to remove all residual traces of dirt and surface impurities.

Various pretreatments depending on the substrate.

Placed into the chrome plating vat and allowed to warm to solution temperature.

Plating current applied and component is left for the required time to attain thickness.

There are many variations to this process depending on the type of substrate being plated upon. Different etching solutions are used for different substrates. Hydrochloric, hydrofluoric, and sulfuric acids can be used. Ferric chloride is also popular for the etching of Nimonic alloys. Sometimes the component will enter the chrome plating vat electrically live. Sometimes the component will have a conforming anode either made from lead/tin or platinized titanium. A typical hard chrome vat will plate at about 25 micrometres (0.001 inches) per hour. To put that into perspective a human hair is between 50 to 100 micrometres.

Chromium plating solutions

Industrial chromium plating is also known as “Hard Chrome” or “Engineered Chrome”. There are two types of Industrial chrome plating solutions:

Hard chromium layers (over 10 micrometres) can be used in various applications and consequently subject to different types of quality requirements. Hard chromium layers on piston rods of hydraulic cylinders are tested on corrosion resistance in salt spray cabinets. Because these are destructive tests, only representative sample material can be tested. The salt spray solutions and the conditions in the cabinet are normed as well as the evaluation of the result after the test. The duration of the test is depending the agressivity of the test and the standard the industry has developed for this type of materials. Typically for engineering purposes the hardness value will be between 800 – 1000 HV500 when subject to a Vickers hardness test. In general there is a requirement that the deposit be uniform in thickness on all surfaces, and should be smooth, homogeneous and free from frosty areas, pin holes, pits, nodules, and other defects.